factors affecting strength and durability of transportation research record 1234 13 factors...
Click here to load reader
Post on 24-Apr-2020
Embed Size (px)
TRANSPORTATION RESEARCH RECORD 1234 13
Factors Affecting Strength and Durability of Concrete Made with Various Cements
K. RosE, B. B. HoPE, AND A. K. C. IP
This investigation examined variables influencing the 28-day com- pressive strength and SO-cycle salt scaling loss of concretes made with 18 Type 10 cements. Statistical analysis was performed on test data consisting of chemical and physical properties of cements; properties of fresh concretes; compressive strength, salt scaling loss, and air void parameters of mature concretes. For a similar water-cement ratio and cement content, results from the corre- lation analysis indicated that the 28-day concrete strength and 50- cycle salt scaling loss were influenced significantly by the chemical and physical properties of the cement used in the mix. Compressive strength has a strong negative correlation with alkali content, indicating that cements with a high alkali content produced con- cretes with lower compressive strength. Fineness (percent of par- ticles in the 4 to 20-µm range) is related to low salt scaling loss. Equations predicting strength and salt scaling loss of concrete were developed by using multiple linear regression.
It has been observed for some time that the quality of the concrete used in Ontario has shown considerable variation, even though all the cements used in the manufacture of con- crete met the Ontario Provincial Standard Specifications Form 1301 (CSA standard CAN 3-A5-M83) requirements for Type 10 cements. As a result of the observed variation in concrete quality in Ontario, a program of testing (J) was undertaken by the Concrete Section in the Engineering Materials Office of the Ontario Ministry of Transportation (MTO). First, phys- ical and chemical properties of 18 samples of cement from 14 different cement plants were measured. These cements were then used to produce samples of concrete with nominal com- pressive strengths of 20 and 30 MP a, respectively. Within each of these strength categories two types of coarse aggregate were used in the mix, a good-quality crushed dolomitic lime- stone called A and a poorer-quality partially crushed natural gravel called B. Various properties of these four resulting concrete types (20A, 20B, 30A and 30B) were also measured.
The experimental investigation was designed to examine the influence of various cements on the strength and durability of concrete. Traditional factors such as cement content and water-cement ratio were not intended to be variables. These two factors have a profound influence on the strength and durability of concretes made from a single cement. Within each of the four concrete types examined in this experiment, all used the same aggregate, had the same cement content, and had virtually the same water-cement ratio. For example, the 30A concretes had the following batch quantities:
Department of Civil Engineering, Queen's University, Kingston, Ontario, Canada K7L 3N6. A. K. C. Ip, current affiliation: Trow, Inc., Brampton, Ontario, Canada K7L 3N6.
Fine aggregate, 37.3 kg; coarse aggregate, 53.7 kg; cement, 17.75 kg; and WRDA, 78.3 ml. DAREX AEA was adjusted to give an air content of 6.0 percent and total water was adjusted to give a slump of 80 mm.
The four concrete types had the same components so that the effect of the cements alone could be studied. This paper is based on a statistical analysis of the test data and was under- taken to address three objectives:
1. Verify that there was a significant difference between the quality of the concretes produced by the various cements.
2. Identify the cement properties responsible for the observed variations in the quality of the concrete specimens.
3. Develop a methodology to help predict the quality of a concrete produced by a cement.
It was decided that the quality of the concrete should be assessed in terms of the compressive strength of the concrete (CSA standard A23.2-3C, 9C) and also the cumulative mass loss (mass of material lost from surface) in a salt scaling test (ASTM C672-84, using 3 percent sodium chloride solution as the de-icer), since these properties most closely reflect the concerns expressed about the durability of concrete. Strength was measured at 3, 7, 28, and 91 days, and salt scaling loss was measured at 5, 10, 15, 25, and 50 cycles. It was decided that the 28-day compressive strength and the 50-cycle salt scaling loss would be the most appropriate variables to use. Therefore, for the purposes of this analysis, these two vari- ables (for each of the four types of concrete) were considered to be the dependent variables. A more detailed description of the analyses reported in this paper is available (2).
The MTO data have been reported (J) in the form of 12 tables labeled A through L. These tables included measurements of chemical and physical properties of the cements, measurements made on the fresh concrete, and measurements made on the mature concretes. These variables are defined in Table 1.
Table C of the MTO data contained the grading curves for the cements. The original 13 variables showed the percent passing specified sieve sizes. It was decided to augment these data by calculating the percentage of cement between two sieve sizes that was passing the larger sieve but retained by the smaller. This step resulted in 42 additional variables. Because the data are highly correlated, only one or two were
TABLE 1 VARIABLES AND DEFINITIONS AND TEST METHODS
VARIABLE DEFINITION/TEST METHOD
Air void content (total)
Chord length (total)
Effective water-cement ratio
Measured at time of casting (%)
Measured on hardened concrete (%)
Na20 + 0.658(K20) (%)
Al 2o3 content of cement (%)
[L .O. I . (at 1050 °C) - L.O. I.
(at 550 °C)] limestone (L.O.I.)] (%)
Cement content per m3 concrete (kg/m3)
Determined by ASTM C457-82a (mm)
CSA Standard CAN 3-A23.2-M77 (kg/m3)
Mass of water/mass of cement
Effective water-cement ratio* Mass of water/mass of cement finer than 45 µm
Fineness (% passing xx µm)
Fineness (% between x-yy µm)
Free calcium oxide
Loss on ignition
Paste-air ratio (total)
Relative density, cement
Spacing factor (total)
Specific surface area
Strength x-day, cement
Strength x-day, concrete
Voids per 25 mm (total)
Void specific surface ( total)
CSA Standard CAN 3-A5-M83 (%)
Fe203 content of cement (%)
Cement finer than xx µm
Cement between x and yy sizes (%)
ASTM Cll4-83a (%)
CSA Standard CAN 3-A5-M83 (%)
CSA Standard CAN 3-A5-M83 (at 1050 °C)(%)
Measured on hardened concrete
K2o content of cement (%)
CSA Standard CAN 3-A5-M83
Measured on hardened concrete (mm)
Calculated from cement grading (mm- 2)
CSA Standard CAN 3-A5-M83 (min)
Si02 content of cement (%)
CSA Standard CAN 3-A23.3-M77 (mm)
Le Chatelier Test (% expansion)
CSA Standard CAN 3-A5-M83 at x days (MPa)
CSA Standard CAN 3-A23.2-M77 at x days (MPa)
so3 content of cement
C4AF content of cement (%)
Calculated c3A content of cement
Calculated c3s content of cement
Measured on hardened concrete
Measured on hardened concrete (mm" 1)
Rose et al.
used in any models that were developed. Finally, it was decided to include the calculated total specific area of the cements as a variable. This variable was included because its calculation made use of all the data in the grading curve.
Table D contained the results of 19 chemical tests per- formed on the cements. In addition, the data were used to calculate three more variables (the percentage of C3S, C2S, and C4AF) thought to be of possible relevance.
The first stage in the analysis was to verify that the observed variation in the measured strength and salt scaling loss for the various concretes was not due to chance alone. The 28- day compressive strength of each concrete sample was mea- sured for four cylinders, and the 50-cycle salt scaling loss for each concrete sample was measured on two cylinders. From these data an analysis of variance was undertaken to test if the variation in results was caused by the various cements. The results of this analysis are summarized in Table 2.
These results show that in all cases there is better than a 99.5 percent confidence (i.e., the probability that the Fvalues could occur by chance is less than 0.005) that the cements differ in their effects on the observed compressive strength and salt scaling loss in the concretes. We therefore concluded that the observed differences in quality are real.
The basic step in developing models that can be used to predict concrete quality is to identify the degree of association between a dependent variable and the independent variables. The SYSTAT (3) package of statistical programs was used to ana- lyze the data. The Pearson correlation coefficient provid